Magnetoelectronic and optical properties of nonuniform graphene nanoribbons
arXiv:1512.08415v5 [physics.comp-ph] 8 Aug 2016
Hsien-Ching Chunga,b,∗, Yu-Tsung Lina , Shih-Yang Lina , Ching-Hong Hoc , Cheng-Peng Changc , Ming-Fa Lina,∗ a
Department of Physics, National Cheng Kung University, Tainan 70101, Taiwan Center for Micro/Nano Science and Technology (CMNST), National Cheng Kung University, Tainan 70101, Taiwan c Center for General Education, Tainan University of Technology, Tainan 701, Taiwan b
Abstract The electronic and optical properties of nonuniform bilayer graphene nanoribbons are worth investigating as they exhibit rich magnetic quantization. Based on our numerical results, their electronic and optical properties strongly depend on the competition between magnetic quantization, lateral confinement, and stacking configuration. The results of our calculations lead to four categories of magneto-electronic energy spectra, namely monolayerlike, bilayer-like, coexistent, and irregular quasi-Landau-level like. Various types of spectra described in this paper are mainly characterized by unusual spatial distributions of wave functions in the system under study. In our paper, we demonstrate that these unusual quantized modes lead to the appearance of such diverse magneto-optical spectra. Moreover, the investigation of the density of states in our model leads to the appearance of many prominent symmetric and weakly asymmetric peaks. The almost well-behaved quasiLandau levels exhibit high-intensity peaks with specific selection rules, and the distorted energy subbands present numerous low-intensity peaks without ∗
Corresponding author Email addresses: [email protected]
(Hsien-Ching Chung), [email protected]
(Ming-Fa Lin) Preprint submitted to Journal of LATEX Templates
August 9, 2016
any selection rules. 1. Introduction Graphene, a one-atom-thick hexagonal lattice comprising carbon atoms, was discovered in 2004 . Its superior electronic [2, 3], magnetic , optical , thermal [3, 6], mechanical , and transport [8, 9] properties are of interest because of the fundamental science included and its technical applications [10–13]. However, its gapless feature results in a low on/off ratio (≈ 5) in graphene-based field-effect transistors (FETs) and is an impediment to the development of graphene nanoelectronics . One of the most promising approaches to controlling the electronic and optical properties is to fabricate quasi-one-dimensional (quasi-1D) graphene strips, referred to as graphene nanoribbons (GNRs). Electrical transport experiments have shown that the lateral-confinement-induced gap in GNRs facilitates the fabrication of FETs with high on/off ratios, approximately 107 at room temperature . Four major state-of-the-art fabrication methods, including both top-down and bottom-up methods, have been proposed to achieve large-scale production of GNRs: cutting of graphene [15, 16], unzipping of carbon nanotube (CNT) [17, 18], chemical vapor deposition (CVD) [19, 20], and piecewise linking of molecular precursor monomers [21, 22]. Researchers are constantly in quest of other methods to precisely control the nanoscale width and realize a perfect edge structure. The first three of the aforementioned four methods can be used to successfully fabricate few-layer GNRs and also nonuniform GNRs. In this study, we investigated the rich magnetic quantization of the electronic and optical properties of nonuniform bilayer GNRs. These GNRs comprise two GNRs with different widths (Fig. 1) and can be fabricated through mechanical exfoliation [23, 24], cutting of graphene [25, 26], chemi2
cal unzipping of CNT [17, 27], and CVD [19, 28]. Changes in the edge structure, ribbon width, and stacking configuration can drastically alter the electronic properties of GNRs. There are two achiral edge structures: zigzag and armchair. The energy gaps of armchair GNRs (AGNRs) have been predicted to be inversely proportional to the GNR width [29, 30]. By contrast, zigzag GNRs (ZGNRs) show dispersionless partial flat subbands at the Fermi energy (EF = 0), arising from the edge-localized states [31, 32]. The width-dependent energy gap has been confirmed by conductance [15, 16] and tunneling current measurements , and the existence of the edge-localized states has been verified using scanning tunneling microscopy (STM) [33, 34] and angle-resolved photoemission spectroscopy . There are two typical stackings in GNRs, namely AB and AA stackings. In the AA stacking, all carbon atoms of the hexagonal rings are nearest-neighbors (i.e., positioned on top of each other), whereas in the AB stacking, only half of the atoms are nearest-neighbors, with the remaining half of the atoms being located above and below the empty centers of the hexagonal rings. Bilayer GNRs show two groups of energy subbands, with each group containing both conduction and valence subbands. The onset energies of the subband groups are closely related to the stacking configuration. For the high symmetry AA stacking, both groups are initiated at an energy approximately equal to the vertical nearest-neighbor interlayer interaction, and there is a strong overlap between the valence subbands of the first group and the conduction subbands of the second group. By contrast, for the AB stacking, one group is at the Fermi energy and the other group is displaced by an energy equal to the nearest-neighbor interlayer interaction. Moreover, there is only a weak overlap between the conduction and the valence subbands of the first group .
Figure 1: Nonuniform bilayer GNR with a narrow top layer (red strip) of width Wt and a wide bottom layer (blue strip) of width Wb ; Ds is the distance between their edges.
A uniform perpendicular magnetic field can bunch neighboring electronic states and thereby form highly degenerate Landau levels with quantized cyclotron radii. Magnetic quantization is strongly suppressed by the lateral confinement. The competition between magnetic quantization and lateral confinement leads to a variety of magnetoelectronic structures including partly dispersionless quasi-Landau levels (QLLs), partial flat subbands, and 1D parabolic subbands [37, 38]. The energy dispersions associated with these subbands lead to two types of peaks in the density of states (DOS), symmetric and asymmetric peaks [39–41]. QLLs can be formed for sufficiently wide nanoribbons, and each Landau wave function has a localized symmetric/antisymmetric spatial distribution with a specific number of zero points (quantum number n). The magneto-optical spectra exhibit numerous symmetric and asymmetric absorption peaks. The symmetric absorption peaks originate from inter-QLL transitions and obey the edge-independent magneto-optical selection rule |∆n| = 1 . By contrast, the asymmetric peaks originate from optical transitions among parabolic subbands and satisfy the edge-dependent selection rules [42–44]. When the number of layers is doubled, bilayer GNRs have two groups of QLLs [40, 45, 46], and their onset energies are the same as the zero-field energies. Furthermore, only the intragroup optical transitions occur in the AA stacking, whereas intergroup transitions are also occur in the AB stacking. This difference is derived from the fact that the wave functions of the AA stacking are symmetric or antisymmetric superpositions of the tight-binding functions on different layers. The magnetoelectronic and optical properties of nonuniform bilayer GNRs are directly dependent on the geometric structures, such as the widths of the top and bottom layers (Wt and Wb ), the relative distance between their edges (Ds ), and inner boundaries of the top narrow ribbon (Fig. 1). Four
categories of magnetoelectronic energy spectra are reflected in the DOS, and they involve monolayer-like, bilayer-like, coexistent, and irregular QLLs. The various categories of QLL spectra show distinct optical properties. In particular, the coexistent QLLs can exist only when the widths of the monolayer and bilayer regions are considerably greater than the magnetic length. The QLL wave functions are well behaved, and they give rise to many highintensity absorption peaks with two specific optical selection rules. In GNRs with irregular QLLs, the two subband groups of different layers vary considerably, and the wave functions are seriously distorted and piecewise continuous. Consequently, many low-intensity absorption peaks without any selection rules exist. These feature-rich electronic and optical properties can be experimentally verified, and the nonuniform GNR provides an alternative for understanding the optical properties of other related structures, such as partially overlapping GNRs [47–49], GNR-graphene superlattices , and van der Waals heterostructures [51–53]. 2. Tight-binding model Zigzag and armchair nanoribbons feature similar magneto-optical transitions, thus for the sake of brevity, we focus on the study of nonuniform bilayer AB-stacked ZGNRs to investigate the edge-independent state energy of their QLLs and magneto-optical selection rule. The geometric structure is composed of two ZGNRs of different widths (Fig. 2(a)). The wide bottom and narrow top layers are represented by the heavy black and light red hexagonal lattices, respectively. The primitive unit cell enclosed by the dashed rectangle √ has a periodic length given by Ix = 3b, where b = 1.42 ˚ A is the C–C bond length. The first Brillouin zone is in the region −π/Ix < kx ≤ π/Ix . The carbon atoms on the mth zigzag line of the bottom (top) layer are denoted 6
(a) Geometric structure of a nonuniform bilayer AB-stacked ZGNR. (b) In-
tralayer and interlayer atomic interactions.
1(2) by A1(2) m ’s (filled circles) or Bm ’s (open circles). The superscripts 1 and 2
indicate the top and bottom layers, respectively. There are 2Nb + 2Nt carbon atoms in a unit cell, where Nb (Nt ) is the number of zigzag lines of the bottom (top) layer. The top and bottom layers have widths of Wt = b(3Nt /2 − 1) and Wb = b(3Nb /2 − 1), respectively, and are vertically shifted by a distance of c = 3.35 ˚ A. The layers conform to AB stacking; in other words, the two hexagonal lattices are displaced by a horizontal distance b from each other as viewed from the top. The first zigzag line of the top layer is on the (ds + 1)th zigzag line of the bottom layer, and the distance between the edges of the top and bottom layers is Ds = |b(3ds − 1)/2|. The low-energy electronic properties are dominated by the tight-binding functions of 2pz orbitals. On the basis of the 2Nb + 2Nt tight-binding func-
tions, the nearest-neighbor Hamiltonian can be expressed as H = −γ0
1 B1 |ΦA m ihΦn |
2 B2 |ΦA m ihΦn |
B |ΦA m ihΦn | + H.c..
The Bloch wave function is given by c,v
|Ψ i = +
1 A1m |ΦA m i
m Nt X
2 A2n |ΦA n i
1 1 Bm |ΦB m i
2 Bn2 |ΦB n i
where |ΦA m
i (|ΦB n
i) represents the tight-binding functions associated
with the 2pz orbitals on the mth (nth) site of the first-layer (second-layer) sublattice A1(2) (B 1(2) ). The first term describes only the intralayer atomic interactions between the nearest neighbors in each layer, and the second term pertains to the interlayer atomic interactions. According to the Slonczewski– Weiss–McClure model , the atomic interactions in 2pz orbitals for the AB stacking are the intralayer atomic interactions between the nearest carbon atoms (γ0 = 2.598 eV), and interlayer atomic interactions between A1 and A2 atoms (γ1 = 0.364 eV), B 1 and B 2 atoms (γ3 = 0.319 eV), and A1 and B 2 (A2 and B 1 ) atoms (γ4 = 0.177 eV) (Fig. 2(b)); there is also a chemical shift 1 2 (γ6 = −0.026 eV) . A1m , Bm , A2m , and Bm in Eq. (2) are the amplitudes
of the subenvelope functions on the four distinct sublattices. When a uniform static magnetic field given by B = B0 zˆ is applied perpendicular to the ribbon plane, the effective Hamiltonian can be interpreted as the Peierls substitution Hamiltonian . Each Hamiltonian matrix element becomes the product of the zero-field element and the extra phase factor exp(i2πθmn ), where θmn is expressed as (1/φ0 )
A · dl and is defined
as a line integral of the vector potential A from the mth site to the nth site. 8
Here, A is chosen as (−B0 y, 0, 0) to preserve the translational invariance in the x-direction under the Landau gauge, and φ0 = h/e is the magnetic flux quantum. The diagonalization of the Hamiltonian matrix H yields the energy spectrum E c,v (kx ) and wave functions |Ψc,v i, where the superscripts c and v denote the conduction and valence subbands, respectively. 3. Magnetoelectronic properties The electronic properties of nonuniform bilayer ZGNRs are very sensitive to changes in the relative position between the two layers, ribbon width, interlayer atomic interactions, and magnetic field. There are four categories of magnetoelectronic energy spectra, namely monolayer-like, bilayer-like, coexistent, and irregular QLL spectra. First, when the top layer is insufficiently wide for magnetic quantization and the bottom layer is sufficiently wide for magnetic quantization, the energy spectrum can be regarded as a mixture of two monolayer-like spectra. One monolayer-like spectrum consists of monolayer-like QLLs contributed by the bottom layer, whose width is greater than the magnetic length (lB =
h ¯ /eB0 ). The other monolayer-like spec-
trum comprises the parabolic subbands arising from the top layer, which has a width lesser than lB . The relative position between the two layers plays a crucial role in the mixing of these electronic energy spectra. As the top layer is at the edge of the bottom layer (ds = 0), the Landau orbits near the center of the bottom layer are almost unaffected (Fig. 3(a)). The QLLs are formed around kx = 2/3, and their energies are roughly proportional to √ c,v n B0 , where nc,v = 0, 1, 2, ... is the subband index labeled from the Fermi energy. QLLs with a larger-nc,v have wider Landau orbits and a smaller kx range in the dispersionless energy spectrum. Because of the destruction of inversion symmetry, the energy spectrum is no longer symmetric about the 9
kx = 0 axis (E c,v (kx ) 6= E c,v (−kx )). Apparently, the parabolic subbands at −kx mix with the left-hand side of the QLLs, instead of the right-hand side of QLLs. Furthermore, two pairs of degenerate partial flat subbands are revealed near EF = 0 with an energy spacing ∆UI of 75 meV, and they are one of the main features of bilayer ZGNRs. When the top layer gradually moves to the center, the parabolic subbands shift to the formation center of QLLs (kx = ±2/3, where parabolic subbands become QLLs as the magnetic field grows) and subband mixings are considerably enhanced. In particular, for the case of a center-positioned top layer (ds = 112), the dispersionless QLLs are transformed to irregular oscillatory QLLs with many extra band-edge states (Fig. 3(b)), indicating that the Landau orbits are strongly suppressed (this is discussed later). The dispersionless QLLs can be recovered from the irregular oscillatory QLLs, as the top layer moves to the right edge (ds = 225 in Fig. 3(c)). Furthermore, the parabolic subbands are shifted to the right side of the QLLs. Additionally, the energy spectra for the cases of the leftedge- and right-edge-aligned top layer (Figs. 3(a) and 3(c)) are not symmetric about the kx = 0 axis because of the asymmetry in the geometric structures. The QLL spectrum can be transformed from a monolayer-like spectrum to a bilayer-like spectrum, depending on the top layer width. For an extremely narrow top layer (Nt = 2, Wt < lB , and Wb > lB ), the main magnetoelectronic energy spectrum is the energy dispersions of the bottom layer, including the monolayer-like QLLs and the partial flat subbands at EF = 0 (red curves in Fig. 4(a)). The top layer contributes only two parabolic subbands with band-edge states at the zone boundaries (black curves). With an increase in the top layer width (Nt = 25, Wt ∼ lB , and Wb > lB in Fig. 3(b)), the monolayer-like QLL spectrum is highly distorted, exhibiting serious subband mixing, because of the interlayer atomic interactions. Later, the second
Low-energy magnetoelectronic structures of nonuniform bilayer AB-stacked
ZGNRs with Nb = 250 and Nt = 25 at (a) ds = 0, (b) ds = 112, and (c) ds = 225 for B0 = 30 T. The top view of each configuration is depicted in the gray zones. The circles mark the locations of the electronic states on the nc = 1–3 QLLs at kx = 2/3. The DOSs are presented in (d), (e), and (f). The red triangles indicate the peaks at ω = −75 meV.
group of QLLs starts at the energies of the nearest-neighbor interlayer interactions (±γ1 ) when Wt > lB (Nt = 150 in Fig. 4(b)). The monolayer-like QLL spectrum evolves into a bilayer-like QLL spectrum. The energy spac√ ings between QLLs are reduced, and the B0 dependence of QLL energies no longer holds. It is noteworthy that the two groups of QLLs are mixed with extra parabolic subbands. The parabolic subbands are due to the nonoverlapping regions of the bottom layer, whose width is insufficiently for magnetic quantization. In another extreme case (Fig. 4(c)), the top layer becomes as wide as the bottom layer (Nt = 250 and Wt = Wb > lB ), and consequently the entire bilayer QLL spectrum is obtained; in Fig. 4(c), the QLLs of the c,v first and second group are indexed with nc,v 1 and n2 , respectively.
The monolayer- and bilayer-like QLL spectra can simultaneously exist because the overlapping and nonoverlapping regions are sufficiently wide for quantizing the electronic states. Furthermore, bilayer- and monolayer-like QLLs at positive (negative) wave vectors are obtained at kx < 2/3 and kx > 2/3 (kx < −2/3 and kx > −2/3), respectively (Fig. 5(a)). An extra group of intermediate QLLs is formed, and it shows subband mixing of the monolayer- and bilayer-like QLLs because of the interface between the regions with/without interlayer interactions. The spatial distributions of intermediate states exhibit wave functions at the interface, and they are discussed later. The coexistent QLL spectrum is also sensitive to the top layer position. In the case of the center-positioned top layer (Fig. 5(b)), there are two groups of monolayer-like QLLs, one group of bilayer-like QLLs, and two extra groups of intermediate QLLs, reflecting the special geometric structure of the nonuniform bilayer ZGNR with two interfaces. The DOS, defined as 2
δ[ω−E c,v (kx , nc,v )] (the numeral 2 indicates
the spin), directly reflects the main features of the energy spectra . Two
Figure 4: Magnetoelectronic structures of the nonuniform ZGNRs with Nb = 250 for (a) Nt = 2, (b) Nt = 150, and (c) Nt = 250 at the ribbon center. The red triangles and blue diamonds mark the locations of the the electronic states on the first- and second-group QLLs at kx = 2/3, respectively. (d)–(f) The corresponding DOSs. The red and blue arrows indicate the first- and second-group QLL peaks, respectively.
Figure 5: Coexistence of monolayer- and bilayer-like QLL energy spectra for nonuniform ZGNRs with Nb = 700 and Nt = 300 at (a) ds = 0 and (b) ds = 200. Insets show magnified views of the intermediate QLLs within the red and blue boxes. The red and blue crosses mark the locations of the electronic states at kx = k1 and k2 , respectively. The corresponding DOSs are shown in (c) and (d), where the red circles, green triangles, and blue diamonds indicate the first few monolayer-like QLL peaks, bilayer-like QLL peaks of the first group, and bilayer-like QLL peaks of the second group, respectively.
types of peaks are presented, including symmetric and asymmetric peaks. The symmetric peaks are delta-function-like peaks with two-side-divergent structure at the peak frequency ω (so that the peak is symmetric about the axis of ω). They are the prominent peaks and originate from partial flat subbands and dispersionless QLLs. The asymmetric peaks with oneside-divergent structure are the secondary peaks, and they originate from the band-edge states of parabolic and irregular oscillatory subbands. The edge-aligned narrow top layer partially distorts the QLLs, and therefore, the monolayer-like DOS is almost unaffected (Figs. 3(d) and 3(f)). The highest symmetric peak at EF = 0 originates mainly from the partial flat subbands, and the QLL peak intensity, proportional to the QLL spread range in the momentum space, gradually decreases with an increase in nc,v . The high-intensity QLL peaks are surrounded by asymmetric subpeaks, which are attributed to the extra band-edge states of the mixed subbands. Notably, the symmetric peak of high intensity at ω = −75 meV (marked by the red triangle in Figs. 3(d) and 3(f)) demonstrates one of the characteristics of bilayer ZGNRs. The DOS varies drastically when the top layer moves above the center of the bottom layer. The QLL peaks are strongly suppressed, and most of them are replaced by lower-intensity asymmetric peaks corresponding to the band-edge states of the irregular oscillatory QLLs (Fig. 3(e)). The width of the center-positioned top layer determines whether the DOS is closer to the monolayer- or bilayer-like DOS. Monolayer-like DOS with additional asymmetric subpeaks are revealed for a very narrow top layer (Fig. 4(d)). When the top layer becomes sufficiently wide (Wt > lB in Fig. 4(e)), the frequency spacings between the suppressed QLLs are reduced (red arrows), and the second group of QLLs forms at ±γ1 (blue arrows). At Wt = Wb , the DOS of the bilayer ZGNR is displayed (Fig. 4(f)). The monolayer-like QLL
peaks can concurrently exist with the bilayer-like QLL peaks for nonuniform ZGNRs with Wt > lB and Wb − Wt > lB as shown in Fig. 5(c) (in Fig. 5(d), (Wb − Wt )/2 > lB ). The monolayer-like QLL peaks with wider spacings are indicated by the red circles, and the bilayer-like QLL peaks with narrower spacings are marked by the green triangles and blue diamonds. Their relative peak height is sensitive to the top-layer position; for example, the intensity of the monolayer-like QLL peaks decreases rapidly for the case of centerpositioned top layer (Fig. 5(d)). It is predicted that the optical absorption peaks are contributed by transitions between high-DOS QLLs. The position- and width-dependent DOSs can provide full information on the electronic energy spectra. Special structures are formed or destroyed when the top-layer position changes (0 ≤ ds ≤ 225 in Fig. 6(a)). The highest peak is contributed by the nc,v = 0 QLL and degenerate partial flat subbands. The intensity of the nc = 1 QLL peak gradually decreases, reaches the minimum (ds = 112 indicated by the red curve), and then increases to the maximum (ds = 225). This is due to the change from the dispersionless QLL to the irregular oscillatory QLL. The other peaks disappear and form at certain critical ds ’s values (indicated by the green and blue lines). This is relatively easily observed for the larger-nc QLL peaks since the dispersionless QLLs are thoroughly transformed into irregular oscillatory QLLs. For another structure in the DOS, the ripples originate from many asymmetric peaks pertaining to the band-edge states of the irregular oscillatory QLLs. On the other hand, the DOS is drastically altered as the top-layer width varies in the range of 2 ≤ Nt ≤ 250 (Fig. 6(b)). The intensities of the monolayerlike QLL peaks decrease rapidly and reduce to zero at certain critical widths (green curve). Two groups of QLL peaks with smaller energy spacings are revealed as the top-layer width increases (blue curves). The unusual evolu-
tion of DOS reflects the drastic transformation from a monolayer-like QLL spectrum to a bilayer-like QLL spectrum. Moreover, the distribution of the monolayer and bilayer electronic states are clearly distinguished, facilitating the determination of the geometric-structure-dependent QLL optical transitions. The main characteristics and the interlayer-atomic-interaction-induced evolution of prominent Landau peaks in the DOS can be verified using scanning tunneling spectroscopy (STS), which is an extension of STM  and provides full information about the surface DOS, such as the DOS of silicon [59, 60] and CNTs [61, 62]. The tunneling conductance (dI/dV ) is proportional to the DOS, and therefore, the structures, positions, and intensities of peaks can be resolved. In very wide GNRs, low-frequency symmet√ ric Landau peaks showing nc,v B0 dependence have been observed [63, 64]. The aforementioned four categories of magnetoelectronic energy spectra in nonuniform ZGNRs can be identified through STS measurements of the DOS [33, 63, 65]. Moreover, the variations of the prominent symmetric QLL peaks during a change in the top layer position/width can be observed, including the peak strength, formation/disapperance of peaks, and the transformation from monolayer-like QLLs to bilayer-like QLLs. In particular, the coexistence of monolayer- and bilayer-like QLLs has been evidenced by conductance measurements. Through gate voltage adjustment, strong suppression of the bilayer resistance oscillation has been observed . Wave functions with diverse spatial distributions are crucial for realizing fundamental physical properties, such as charge density [66–69], state mixing , and optical transition [29, 70]. The wave functions of ZGNRs (Eq. (2)) can be decomposed into the subenvelope functions of distinct sublattices
(a) nc,v=0 nc=1 nc=2 c
n =3 nc=4 nc=5
nc=1 nc=2 n =3 c
n1c=4 6 c 2
(a) Position-dependent DOS for the nonuniform ZGNR with Nb = 250 and
Nt = 25. (b) Width-dependent DOS for the nonuniform ZGNR with Nb = 250 and a centered top layer. The DOSs at three characteristic positions (curves 1–3 for ds = 0, 112, and 225) and for three characteristic widths (curves 4–6 for Nt = 2, 150, and 250) are shown in red in Figs. 3(d)–3(f) and Figs. 4(d)–4(f). The geometric configurations for the characteristic positions/widths are indicated by the shaded parallelograms.
as follows: c,v
|Ψ i =
1 A1o |ΦA m i
1 Bo1 |ΦB m i
2 A2o |ΦA m i
2 Bo2 |ΦB m i
1 B 2 A 2 B A1e |ΦA n i + Be |Φn i + Ae |Φn i + Be |Φn i ,
where the subscript o (e) indicates amplitudes on odd (even) zigzag lines. Only the odd terms are discussed because of the phase difference of π (e.g., A1o = −A1e ). In general, the electronic states in the parabolic subbands present standing waves, reflecting the lateral confinement. Furthermore, the quantized states in the dispersionless QLLs show Landau wave functions, which are products of a Hermite polynomial and a Gaussian distribution function. Because the prominent absorption peaks arise from the optical transitions between QLLs, it is worthwhile to investigate the wave functions at the formation center of QLLs. The wave functions are strongly dependent on the position of the narrow top layer. When the top layer is positioned at the edge of the bottom layer, the QLLs remain dispersionless and the center-located Landau wave functions are almost unaffected. The nc = 1–3 Landau wave functions at kx = 2/3 (black circles in Fig. 3(a)) show Landau modes in A1o and Bo1 sublattices, and these modes are similar to those of the monolayer ZGNR (heavy black dots in Fig. 7). Such spatial distributions of Landau modes are either symmetric or antisymmetric, and the node number of the subenvelope functions in sublattice A1o is lower than that in sublattice Bo1 by one. For instance, there are one and two nodes on the A1o and Bo1 sublattices for the nc = 2 QLL, respectively (Figs. 7(b1) and 7(b2)). Therefore, the subband of the larger state energy |E c,v | has a larger node number, and the number of nodes on the Bo1 sublattice is chosen to be suitable for indexing the subbands. The electronic states are drastically altered by interlayer atomic interactions. 19
Figure 7: Wave functions of the subbands corresponding to the nc range 1–3 at kx = 2/3. Heavy black dots denote the top layer of width Nt = 25 at ds = 0, and light red dots correspond to Nt = 25 and ds = 112. The gray zones indicate the centered top layer.
The states of the nc = 1–3 irregular oscillatory QLLs at kx = 2/3 (red circles in Fig. 3(b)) are mixed with the states of parabolic subbands, and therefore, the wave functions (light red dots in Fig. 7) become piecewise continuous or have two jump discontinuities in the A1o and Bo1 sublattices at the two edges of the top ribbon (edges of gray zone), indicating the absence of the normal Landau modes. Furthermore, the spatial distributions of the top layer (A2o and Bo2 ) turn out to be observable, showing distorted standing waves. It is predicted that the suppression of QLL transition peaks and the appearance of additional subpeaks occurs because of the distortions in wave functions.
The monolayer-like Landau wave functions evolve into bilayer-like Landau wave functions when the top layer of the nonuniform GNR becomes sufficiently wide. In the uniform bilayer ZGNRs (Wb = Wt ), the spatial distributions of Landau wave functions, including the amplitude, spatial symmetry, and node number, are not well behaved under the influence of interlayer interactions. In both groups of Landau states, the wave functions at the formation center are somewhat distorted and the amplitudes are different for the four sublattices (heavy black dots in Fig. 8). Obviously, in the first-group (second-group) Landau states, the amplitude of the Bo1 (A1o ) sublattice dominates among the amplitudes of the four sublattices, and the corresponding node number is characterized as the subband index. In other c,v words, for the nc,v 1 = n ≥ 2 (n2 = n ≥ 1) Landau wave functions, there
are n − 1, n, n − 1, and n − 2 (n, n + 1, n, and n − 1) nodes in the subenvelope functions of sublattices A1o , Bo1 , A2o , and Bo2 , respectively. For the nonuniform ZGNR with a sufficiently wide top layer (Wb > Wt > lB ), the QLL wave functions are similar to those of bilayer ZGNRs (light red dots in Fig. 8). The regularity of node numbers in the Landau modes and the dominant sublattices for each group remain the same. However, the Landau wave functions of the second group have an extra component—the standing waves of parabolic subbands—and therefore show slightly distorted distributions (Figs. 8(a) and 8(b)). It is predicted that there are four categories of inter-QLL transitions, two intragroup and two intergroup transitions. For the nonuniform GNR with sufficiently wide overlapping and nonoverlapping regions, the monolayer and bilayer Landau wave functions can concurrently exist. At the formation center of monolayer-like QLLs (kx = k1 ), the features of Landau wave functions are identical to those of the QLLs in monolayer ZGNR. The symmetric/antisymmetric subenvelope functions
Figure 8: Wave functions of the low-lying QLLs at kx = 2/3. The light red dots denote the centered top layer of width Nt = 150, and the heavy black dots represent the centered top layer of width Nt = 250. The gray zones indicate the centered top layer with Nt = 150. The locations of the electronic states on the first- and second-group QLLs are marked by the red triangles and blue diamonds in Fig. 4, respectively.
of sublattices A1o and Bo1 are localized at the center of the nonoverlapping region (white zones in Figs. 9(a1), 9(a2), 9(b1), 9(b2), 9(c1), and 9(c2)), and their node numbers are n − 1 and n for the nc,v = n monolayer-like QLLs, respectively. Meanwhile, at the formation center of bilayer-like QLLs (kx = k2 ), Landau wave functions of the bilayer ZGNR are exhibited. The slightly distorted subenvelope functions are localized at the center of the overlapping region (Figs. 9(d)–9(f)), and the node number in each sublattice is identical to that of the bilayer ZGNR. In addition, near the interface between the two regions, the wave functions are distributed in a piecewise continuous form and the distorted bilayer and monolayer Landau wave functions are joined . The prominent absorption spectrum is predicted to be characterized by optical transitions between the monolayer-like QLLs and between the bilayer-like QLLs. The aforementioned features of wave functions can be investigated by spectroscopic-imaging STM [72–74]. It can resolve charge distributions from the local DOS and is a powerful tool for identifying standing waves and Landau wave functions on the surfaces of various condensed-matter systems. Standing waves have been directly observed at the surface steps of Au(111) and Cu(111) [72, 75]. Furthermore, theoretical predictions of the standing waves in a finite-length metallic CNT [76, 77] have also been verified [62, 78]. Recently, Landau orbits without the zero point have been observed [79, 80], and subsequently, observations of the concentric-ring-like nodal structures have also been made [81, 82]. In nonuniform GNRs, the monolayer/bilayer/distorted Landau wave functions are closely related to the geometric configuration. In particular, interlayer interactions lead to state mixing, and interfaces give rise to the discontinuous distributions. The diverse spatial distributions in Landau wave functions can be examined through
Figure 9: Wave functions of the low-lying subbands at kx = k1 and k2 . The shaded regions represent the top layer of width Nt = 300 at ds = 0. The locations of the electronic states at kx = k1 and k2 are indicated by the red and blue crosses in Fig. 5(a), respectively.
spectroscopic-imaging STM measurements on nodal structures. 4. Magneto-optical properties When a GNR is placed in an electromagnetic field with the electric polarˆkˆ ization e x, electrons are excited from occupied to unoccupied states. Vertical optical excitations with the same wave vector (∆kx = 0) are available since the photon momentum is almost zero. The optical absorption function based on Fermi’s golden rule is given by A(ω) ∝
h,h0 =c,v n,n0
dkx f [E h (kx , n0 )] − f [E h (kx , n)] Im 2π E h0 (kx , n0 ) − E h (kx , n) − ω − iΓ
2 ˆ · p h h0 0 e Ψ (kx , n ) Ψ (kx , n) , me
where me is the bare electron mass, p is the momentum operator, f [E h (kx , n)] is the Fermi–Dirac distribution function, and Γ (≈ 2 meV) is the phenomenological broadening parameter. The spectral intensity is dominated by the joint DOS (the first term) and the velocity matrix element (the second term). The second term is evaluated within the gradient approximation [83– 85]; such evaluation has previously been successfully performed for layered graphite [84, 86], CNTs [86, 87], and few-layer graphenes [88, 89]. The velocity matrix element is expressed as (1/¯h)
Clh ∗ (kx , n0 )Clh0 (kx , n)[∂Hl,l0 (kx )/∂kx ],
where Clh0 (kx , n) is the amplitude at the lattice site of the subenvelope function. The nonvanishing ∂Hl,l0 /∂kx is related to the nearest-neighbor atomic interactions. The presence of optical transitions depends on the finite inner product among the initial state and final state on different sublattices and ∂Hl,l0 /∂kx . For example, the edge-dependent optical selection rules for GNRs in the absence of external fields have been obtained by analyzing the velocity matrix elements and the special relationships among wave functions. The 25
selection rules are |∆J| = odd for ZGNRs and ∆J = 0 for AGNRs, where J is the subband index [42, 44]. On the basis of the geometric configuration, the magnetoabsorption spectra of nonuniform GNRs can be divided into four categories: monolayer-like, bilayer-like, coexistent, and irregular spectra. The prominent QLL transition peaks might be strongly suppressed, depending on the position of the narrow top layer. For an edge-aligned top layer (Figs. 10(a) and 10(c)), the magnetoabsorption spectrum is very similar to that of monolayer ZGNRs (light red curve), except for few extra subpeaks. There are many prominent symmetric peaks (ωnv nc ’s) associated with the vertical transitions from the nv QLL to the nc = nv ± 1 QLL. This is because valence and conduction subbands with adjacent indices possess the same Landau mode. The velocity matrix elements have finite values, and therefore, the optical transitions can exist for the subbands satisfying the magneto-optical selection rule |∆n| = |nc − nv | = 1 [39, 70]. Furthermore, the peak height, which is proportional to the kx range of the QLL, decreases with an increase in the frequency. Notably, the QLL transition frequencies exhibit the simple √ √ √ √ relation B0 ( nv + nv ± 1) based on the nc,v B0 relationship and the selection rule |∆n| = 1. The extra absorption subpeaks originate from the transitions between the band-edge states of mixed subbands. In particular, the number, intensity, and frequency of the absorption peaks are very sensitive to the position of the top layer, especially for a center-positioned top layer (Fig. 10(b)). Most of the higher-frequency peaks are thoroughly suppressed because of distortions in the wave functions, whereas the intensity of the low-frequency peaks is reduced. The top-layer width dominates whether the QLL spectrum is a monolayerlike spectrum or bilayer-like spectrum. Monolayer-like QLLs are exhibited in
Figure 10: Low-frequency magneto-optical absorption spectra of the nonuniform ZGNRs with Nb = 250 and Nt = 25 at (a) ds = 0, (b) ds = 112, and (c) ds = 225 for B0 = 30 T. Light red curve indicates the magnetoabsorption spectrum of the monolayer ZGNR. Dashed red lines indicate the inter-QLL absorption frequencies of the monolayer ZGNR.
the nonuniform GNR with a very narrow top layer (Fig. 11(a)). The intensity of the QLL transition peaks is lower for a wider top layer (Fig. 11(b)). When the top ribbon width is close to the spatial distribution of Landau wave functions (Nt = 100 in Fig. 11(c)), the interlayer interactions strongly suppress the QLL transition peaks, lead to the absence of selection rules, and cause many low-intensity subpeaks to appear. The main reason is that the dispersionless QLLs become irregular oscillatory QLLs, and the wave functions are highly distorted. However, two groups of QLLs are formed as the top layer width is sufficient for magnetic quantization (e.g., Nt = 150 in Fig. 4(b)). Consequently, the absorption spectrum (Nt = 150 in Fig. 11(d)) is similar to that of the bilayer (Wt = Wb in Fig. 11(e)). There are four categories of inter-QLL absorption peaks, and half of them belong to intragroup or intergroup excitations. In particular, the low-frequency peaks originate from the intragroup QLL transitions (ωn1 c1 nv1 ) between the nc1 and nv1 QLLs. These peaks obey the selection rule |∆nintra | = |nc1 − nv1 | = 1 because the Landau modes are the same on the ith layer for the Ai (B i ) sublattice of the initial state and the B i (Ai ) sublattice of the final state [36, 90]. Because of the 1 1 asymmetric QLL spectrum, the intragroup transitions (ωn(n−1) and ω(n−1)n ) 1 show twin-peak structures, except for the threshold transitions (ω12 ).
Monolayer and bilayer QLL transitions can exist simultaneously when the nonoverlapping and overlapping regions are sufficiently wide for the quantization of the electronic states. The well-behaved monolayer and bilayer Landau wave functions are in the nonoverlapping and overlapping regions, respectively (Fig. 9), and therefore, the different optical transitions can concurrently exist. The |∆n| = 1 absorption peaks with wide frequency spacings and the |∆nintra | = 1 peaks with narrower frequency spacings are clearly present in Fig. 12. Moreover, their relative peak height is roughly propor-
Figure 11: Magneto-optical absorption spectra of the nonuniform ZGNRs with Nb = 250 for (a) Nt = 2, (b) Nt = 25, (c) Nt = 100, (d) Nt = 150, and (e) Nt = 250 at the ribbon center. Dashed red and blue lines represent the inter-QLL absorption frequencies of the monolayer and bilayer ZGNRs, respectively.
Magneto-optical spectrum of the nonuniform ZGNR with Nb = 700 and
Nt = 300 at ds = 0.
tional to the ratio between the widths of the two distinct regions. The inter-QLL transitions and selection rules can be examined through experimental measurements, as previously performed for few-layer graphenerelated systems by using magneto-optical transmission [91, 92] and magnetoRaman spectroscopy . Some of the theoretical predictions, especially regarding the threshold absorption peak of ω01 in a magnetic-field, of GNRs have been recently verified through infrared transmission measurement on epitaxial monolayer GNR arrays . For narrow monolayer GNRs, ω01 does √ not obey the B0 dependence at low magnetic fields. However, the dependence is satisfied at high magnetic fields. The predicted magneto-optical properties of nonuniform GNRs can be verified, and they include the monolayer, bilayer, and coexistent QLL absorption spectra, magneto-optical selec30
tion rules, and single-peak, twin-peak, and irregular-peak structures. They are quite sensitive to the geometric configuration. Moreover, the discussions presented provide an elementary example for understanding the optical properties of other similar structures and the effect of van der Waals interactions, such as partially overlapping GNRs [47–49], GNR-graphene superlattices , and van der Waals heterostructures [51–53]. 5. Conclusion The low-energy magnetoelectronic and optical properties of nonuniform bilayer GNRs can be considerably altered by changing their geometric configuration. There are four categories of QLL spectra: monolayer-like, bilayerlike, coexistent, and irregular oscillatory spectra. Monolayer-like QLLs are revealed for an edge-aligned narrow top layer (Wt < lB ), for which the Landau wave functions have almost well-behaved modes. The prominent symmetric DOS peaks arise from the QLLs and partial flat subbands. With an increase in the width of the top layer, the QLLs evolve from dispersionless to irregular oscillatory and show many extra band-edge states. Furthermore, interlayer atomic interactions induce considerable distortions in wave functions and severe state mixing between parabolic subbands and QLLs. The major symmetric DOS peaks are suppressed, and additional asymmetric subpeaks related to the extra band-edge states are revealed. A bilayer-like QLL spectrum is formed when the top layer is sufficiently wide (Wt > lB ) for the quantization of the electronic states. There are two groups of QLLs and symmetric DOS peaks. Furthermore, the Landau wave functions become bilayer-like wave functions because of interlayer interactions. For nonuniform GNRs with sufficiently wide nonoverlapping and overlapping regions, monolayer- and bilayer-like QLLs concurrently exist; moreover, DOS peaks 31
are also revealed. The well-behaved monolayer and bilayer Landau states are present in the nonoverlapping and overlapping regions, respectively. The main characteristics of electronic properties revealed in the DOS and wave functions can be identified by using STS and spectroscopic-imaging STM. Unusual electronic structures are reflected in the absorption spectra. The low-frequency prominent symmetric absorption peaks corresponding to the inter-QLL transitions obey the magneto-optical selection rule |∆n| = 1 for monolayer-like QLLs and |∆nintra | = 1 for bilayer-like QLLs. In the disordered QLL spectrum, higher-frequency inter-QLL transitions are suppressed, and many low-intensity peaks without selection rules are revealed. In particular, monolayer- and bilayer-like absorption spectra can coexist when the widths of both nonoverlapping and overlapping regions are sufficiently wide for magnetic quantization. The feature-rich absorption spectra and selection rules can be explored using magneto-optical transmission and magnetoRaman spectroscopy.
Recently, partially overlapping structures between
CVD-grown graphene grains have been synthesized [47, 49, 94]. The theoretical study of nonuniform GNRs can provide an essential understanding of such structures and the effective van der Waals interactions have on their properties. Acknowledgements We would like to thank all the contributors to this article for their valuable discussions and recommendations, especially Ming-Hsun Lee, Po-Shin Shi, Thi-Nga Do, Ngoc Thanh Thuy Tran, Matisse Wei-Yuan Tu, PingYuan Lo, Yu-Ming Wang, Hao-Chun Huang, and Kuan-Yu Chen. The authors thank Pei-Ju Chien for English discussions and corrections. One of us (Hsien-Ching Chung) thanks Ming-Hui Chung and Su-Ming Chen for fi32
nancial support. This research received funding from the Headquarters of University Advancement at the National Cheng Kung University, which is sponsored by the Ministry of Education, Taiwan. This work was supported in part by the National Science Council of Taiwan under grant number NSC 102-2112-M-006-007-MY3. References References  Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, et al. Electric field effect in atomically thin carbon films. Science 2004;306(5696):666. doi:10.1126/science.1102896.  Berger C, Song ZM, Li XB, Wu XS, Brown N, Naud C, et al. Electronic confinement and coherence in patterned epitaxial graphene. Science 2006;312(5777):1191. URL: ://WOS:000237957400047. doi:10.1126/science.1125925.  Morozov SV, Novoselov KS, Katsnelson MI, Schedin F, Elias DC, Jaszczak JA, et al. Giant intrinsic carrier mobilities in graphene and its bilayer. Physical Review Letters 2008;100(1):016602. URL: : //000252285500055. doi:01660210.1103/PhysRevLett.100.016602.  Lai YH, Ho JH, Chang CP, Lin MF. Magnetoelectronic properties of bilayer bernal graphene. Physical Review B 2008;77(8):085426. URL: ://WOS:000253764300109. doi:08542610.1103/PhysRevB. 77.085426.  Nair RR, Blake P, Grigorenko AN, Novoselov KS, Booth TJ, Stauber T, et al. Fine structure constant defines visual transparency of graphene. 33
Science 2008;320(5881):1308. URL: ://000256441100035. doi:10.1126/science.1156965.  Balandin AA, Ghosh S, Bao WZ, Calizo I, Teweldebrhan D, Miao F, et al. Superior thermal conductivity of single-layer graphene. Nano Letters 2008;8(3):902. URL: ://WOS:000253947400025. doi:10. 1021/nl0731872.  Lee C, Wei XD, Kysar JW, Hone J.
Measurement of the elas-
tic properties and intrinsic strength of monolayer graphene. Science 2008;321(5887):385.
URL: ://000257713900044. doi:10.
1126/science.1157996.  Novoselov KS, Geim AK, Morozov SV, Jiang D, Katsnelson MI, Grigorieva IV, et al. Two-dimensional gas of massless dirac fermions in graphene. Nature 2005;438(7065):197. doi:10.1038/nature04233.  Novoselov KS, Jiang Z, Zhang Y, Morozov SV, Stormer HL, Zeitler U, et al. Room-temperature quantum hall effect in graphene. Science 2007;315(5817):1379. URL: ://WOS:000244752200023. doi:10.1126/science.1137201.  Su YH, Wu YK, Tu SL, Chang SJ. Electrostatic studies of pi-pi interaction for benzene stacking on a graphene layer. Applied Physics Letters 2011;99(16):163102. doi:10.1063/1.3653284.  Fo`a Torres LEF, Perez-Piskunow PM, Balseiro CA, Usaj G. Multiterminal conductance of a floquet topological insulator. Physical Review Letters 2014;113(26):266801. doi:10.1103/PhysRevLett.113.266801.  Su YH, Huang SH, Kung PY, Shen TW, Wang WL.
generation of cu2o nanoparticles/mno-mno2 nanorods heterojunction 34
supported on sonochemical-assisted synthesized few-layer graphene in water-splitting photocathode. ACS Sustainable Chemistry and Engineering 2015;3(9):1965. doi:10.1021/acssuschemeng.5b00579.  Wu HC, Chaika AN, Huang TW, Syrlybekov A, Abid M, Aristov VY, et al.
Transport gap opening and high on-off current ratio in tri-
layer graphene with self-aligned nanodomain boundaries. ACS Nano 2015;9(9):8967.
URL: ://WOS:000361935800035. doi:10.
1021/acsnano.5b02877.  Xia F, Farmer DB, Lin Ym, Avouris P. Graphene field-effect transistors with high on/off current ratio and large transport band gap at room temperature. Nano Letters 2010;10(2):715. URL: ://WOS: 000274338800060. doi:10.1021/nl9039636.  Li XL, Wang XR, Zhang L, Lee SW, Dai HJ.
derived, ultrasmooth graphene nanoribbon semiconductors.
ence 2008;319(5867):1229. URL: ://WOS:000253530600039. doi:10.1126/science.1150878.  Han MY, Ozyilmaz B, Zhang YB, Kim P. gap engineering of graphene nanoribbons.
Physical Review Let-
ters 2007;98(20):206805. URL: ://WOS:000246624000056. doi:10.1103/PhysRevLett.98.206805.  Kosynkin DV, Higginbotham AL, Sinitskii A, Lomeda JR, Dimiev A, Price BK, et al. Longitudinal unzipping of carbon nanotubes to form graphene nanoribbons. Nature 2009;458(7240):872. URL: : //WOS:000265182500039. doi:10.1038/nature07872.
 Cataldo F, Compagnini G, Patane G, Ursini O, Angelini G, Ribic PR, et al.
Graphene nanoribbons produced by the oxidative un-
zipping of single-wall carbon nanotubes.
URL: ://000278585400027. doi:10.1016/j.carbon.2010. 03.063.  Campos-Delgado J, Romo-Herrera JM, Jia XT, Cullen DA, Muramatsu H, Kim YA, et al. Bulk production of a new form of sp(2) carbon: Crystalline graphene nanoribbons. Nano Letters 2008;8(9):2773. URL: ://WOS:000259140200030. doi:10.1021/nl801316d.  Sprinkle M, Ruan M, Hu Y, Hankinson J, Rubio-Roy M, Zhang B, et al.
Scalable templated growth of graphene nanoribbons on
sic. Nature Nanotechnology 2010;5(10):727. URL: ://WOS: 000282578000011. doi:10.1038/nnano.2010.192.  Cai JM, Ruffieux P, Jaafar R, Bieri M, Braun T, Blankenburg S, et al. Atomically precise bottom-up fabrication of graphene nanoribbons. Nature 2010;466(7305):470. URL: ://WOS:000280141200031. doi:10.1038/nature09211.  Yi Z, Yanfang Z, Geng L, Jianchen L, Xiao L, Shixuan D, et al. Direct visualization of atomically precise nitrogen-doped graphene nanoribbons. Applied Physics Letters 2014;105(2):023101. URL: : //INSPEC:14430135. doi:10.1063/1.4884359.  Puls CP, Staley NE, Liu Y. Interface states and anomalous quantum oscillations in hybrid graphene structures.
Physical Review B
 Tian J, Jiang Y, Childres I, Cao H, Hu J, Chen YP. Quantum hall effect in monolayer-bilayer graphene planar junctions. Physical Review B 2013;88(12):125410. doi:10.1103/PhysRevB.88.125410.  Tapaszto L, Dobrik G, Lambin P, Biro LP. Tailoring the atomic structure of graphene nanoribbons by scanning tunnelling microscope lithography. Nature Nanotechnology 2008;3(7):397. URL: ://WOS: 000257984700010. doi:10.1038/nnano.2008.149.  Fujii S, Enoki T. Cutting of oxidized graphene into nanosized pieces. Journal of the American Chemical Society 2010;132(29):10034. URL: ://WOS:000280227700037. doi:10.1021/ja101265r.  Kosynkin DV, Lu W, Sinitskii A, Pera G, Sun ZZ, Tour JM. Highly conductive graphene nanoribbons by longitudinal splitting of carbon nanotubes using potassium vapor. ACS Nano 2011;5(2):968. doi:10. 1021/nn102326c.  Wei DC, Liu YQ, Zhang HL, Huang LP, Wu B, Chen JY, et al. Scalable synthesis of few-layer graphene ribbons with controlled morphologies by a template method and their applications in nanoelectromechanical switches. Journal of the American Chemical Society 2009;131(31):11147. doi:10.1021/ja903092k.  Barone V, Hod O, Scuseria GE. Electronic structure and stability of semiconducting graphene nanoribbons. Nano Letters 2006;6(12):2748. URL: ://WOS:000242786500020. doi:10.1021/nl0617033.  Abergel DSL, Apalkov V, Berashevich J, Ziegler K, Chakraborty T. Properties of graphene: a theoretical perspective. Advances in Physics
URL: ://WOS:000280611900001. doi:10.
1080/00018732.2010.487978.  Fujita M, Wakabayashi K, Nakada K, Kusakabe K. Peculiar localized state at zigzag graphite edge. Journal of the Physical Society of Japan 1996;65(7):1920. URL: ://WOS:A1996VA31300012.  Brey L, Fertig HA. Electronic states of graphene nanoribbons studied with the dirac equation. Physical Review B 2006;73(23):235411. URL: ://WOS:000238696600133. doi:10.1103/PhysRevB. 73.235411.  Kobayashi Y, Fukui K, Enoki T, Kusakabe K, Kaburagi Y. Observation of zigzag and armchair edges of graphite using scanning tunneling microscopy and spectroscopy. Physical Review B 2005;71(19):193406. URL: ://WOS:000230244100025. doi:10.1103/PhysRevB. 71.193406.  Li YY, Chen MX, Weinert M, Li L. Direct experimental determination of onset of electron-electron interactions in gap opening of zigzag graphene nanoribbons. Nature Communications 2014;5:4311. URL: : //WOS:000340615500002. doi:10.1038/ncomms5311.  Sugawara K, Sato T, Souma S, Takahashi T, Suematsu H. Fermi surface and edge-localized states in graphite studied by high-resolution angle-resolved photoemission spectroscopy.
Physical Review B
2006;73(4):045124. URL: ://WOS:000235009700041. doi:10. 1103/PhysRevB.73.045124.  Chung HC, Chang CP, Lin CY, Lin MF. Electronic and optical prop-
erties of graphene nanoribbons in external fields. Physical Chemistry Chemical Physics 2016;18(11):7573. doi:10.1039/c5cp06533j.  Wakabayashi K, Fujita M, Ajiki H, Sigrist M. Electronic and magnetic properties of nanographite ribbons. Physical Review B 1999;59(12):8271. URL: ://WOS:000079514300069.  Ostahie B, Nita M, Aldea A. Electrical manipulation of edge states in graphene and the effect on quantum hall transport. Physical Review B 2015;91(15):155409.
doi:10.1103/PhysRevB.91.155409.  Huang YC, Chang CP, Lin MF. Magnetic and quantum confinement effects on electronic and optical properties of graphene ribbons. Nanotechnology 2007;18(49):495401. doi:10.1088/0957-4484/18/49/495401.  Chung HC, Huang YC, Lee MH, Chang CC, Lin MF. Quasi-landau levels in bilayer zigzag graphene nanoribbons. Physica E 2010;42(4):711. doi:10.1016/j.physe.2009.11.090.  Chung HC, Lee MH, Chang CP, Huang YC, Lin MF. Effects of transverse electric fields on quasi-landau levels in zigzag graphene nanoribbons. Journal of the Physical Society of Japan 2011;80(4):044602. URL: ://WOS:000289346600023. doi:10.1143/jpsj.80.044602.  Hsu H, Reichl LE. Selection rule for the optical absorption of graphene nanoribbons. Physical Review B 2007;76:045418. URL: : //WOS:000248540000112. doi:10.1103/PhysRevB.76.045418.  Lin MF, Shyu FL. Optical properties of nanographite ribbons. Journal of the Physical Society of Japan 2000;69(11):3529–32. URL: : //WOS:000165569400015. 39
 Chung HC, Lee MH, Chang CP, Lin MF.
Exploration of edge-
dependent optical selection rules for graphene nanoribbons. Optics Express 2011;19(23):23350. doi:10.1364/OE.19.023350.  Chung HC, Su WP, Lin MF.
Electric-field-induced destruction of
quasi-landau levels in bilayer graphene nanoribbons. Physical Chemistry Chemical Physics 2013;15(3):868.
000312217200019. doi:10.1039/c2cp43631k.  Chung HC, Yang PH, Li TS, Lin MF.
Effects of transverse elec-
tric fields on landau subbands in bilayer zigzag graphene nanoribbons. Philosophical Magazine 2014;94(16):1859.
000337246100007. doi:10.1080/14786435.2014.897009.  Tsen AW, Brown L, Levendorf MP, Ghahari F, Huang PY, Havener RW, et al. Tailoring electrical transport across grain boundaries in polycrystalline graphene. Science 2012;336(6085):1143. URL: : //WOS:000304647900045. doi:10.1126/science.1218948.  Berahman M, Sanaee M, Ghayour R. A theoretical investigation on the transport properties of overlapped graphene nanoribbons. Carbon 2014;75:411. URL: ://WOS:000336877600043. doi:10.1016/ j.carbon.2014.04.020.  Rao R, Pierce N, Xu Q, Harutyunyan AR. Probing inhomogeneous doping in overlapped graphene grain boundaries by raman spectroscopy. Carbon 2014;80:513.
doi:10.1016/j.carbon.2014.08.091.  Wong JH, Wu BR, Yang PH, Lin MF. Low-energy electronic properties of graphene and armchair ribbon superlattices. 40
Physical Chemistry C 2013;117(14):7326.
000317552200047. doi:10.1021/jp310956a.  Geim AK, Grigorieva IV.
Van der waals heterostructures.
2013;499(7459):419. doi:10.1038/nature12385.  Zheng Z, Zhang X, Neumann C, Emmrich D, Winter A, Vieker H, et al. Hybrid van der waals heterostructures of zero-dimensional and two-dimensional materials. Nanoscale 2015;7(32):13393. doi:10.1039/ c5nr03475b.  Foa Torres LEF, Dal Lago V, Suarez Morell E. Crafting zero-bias oneway transport of charge and spin. Physical Review B 2016;93(7):075438. doi:10.1103/PhysRevB.93.075438.  Wallace PR.
The band theory of graphite.
1947;71(9):622. doi:10.1103/PhysRev.71.622.  Charlier JC, Gonze X, Michenaud JP.
1st-principles study of the
electronic-properties of graphite. Physical Review B 1991;43(6):4579. URL: ://WOS:A1991EY62300003. doi:10.1103/PhysRevB. 43.4579.  Peierls R. Zur theorie des diamagnetismus von leitungselektronen. Z Phys 1933;80:763.  Lo PY, Xiong HN, Zhang WM. Breakdown of bose-einstein distribution in photonic crystals. Scientific Reports 2015;5:9423. doi:10.1038/ srep09423.  Binning G, Rohrer H, Gerber C, Weibel E. Surface studies by scanning tunneling microscopy. Physical Review Letters 1982;49(1):57. URL: 41
://WOS:A1982NV44300017. doi:10.1103/PhysRevLett.49. 57.  Hamers RJ, Tromp RM, Demuth JE.
of si(111)-(7 x 7) resolved in real space.
Physical Review Letters
1986;56(18):1972. URL: ://WOS:A1986C111400023. doi:10. 1103/PhysRevLett.56.1972.  Piancastelli MN, Motta N, Sgarlata A, Balzarotti A, Decrescenzi M.
Topographic and spectroscopic analysis of ethylene adsorption
on si(111)7x7 by stm and sts. Physical Review B 1993;48(24):17892. doi:10.1103/PhysRevB.48.17892.  Wildoer JWG, Venema LC, Rinzler AG, Smalley RE, Dekker C. Electronic structure of atomically resolved carbon nanotubes. ture 1998;391(6662):59.
doi:10.1038/34139.  Venema LC, Wildoer JWG, Janssen JW, Tans SJ, Tuinstra H, Kouwenhoven LP, et al. Imaging electron wave functions of quantized energy levels in carbon nanotubes. Science 1999;283(5398):52. URL: : //WOS:000077976600045. doi:10.1126/science.283.5398.52.  Miller DL, Kubista KD, Rutter GM, Ruan M, de Heer WA, First PN, et al. Observing the quantization of zero mass carriers in graphene. Science 2009;324(5929):924. URL: ://WOS:000266048800034. doi:10.1126/science.1171810.  Song YJ, Otte AF, Kuk Y, Hu Y, Torrance DB, First PN, et al. High-resolution tunnelling spectroscopy of a graphene quartet. Nature 2010;467(7312):185. doi:10.1038/nature09330. 42
 Niimi Y, Kambara H, Matsui T, Yoshioka D, Fukuyama H.
space imaging of alternate localization and extension of quasi-twodimensional electronic states at graphite surfaces in magnetic fields. Physical Review Letters 2006;97(23):236804. URL: ://WOS: 000242708900045. doi:10.1103/PhysRevLett.97.236804.  Schrodinger E. An undulatory theory of the mechanics of atoms and molecules. Physical Review 1926;28(6):1049. doi:10.1103/PhysRev. 28.1049.  Tu MWY, Zhang WM. Non-markovian decoherence theory for a doubledot charge qubit. Physical Review B 2008;78(23):235311. doi:10.1103/ PhysRevB.78.235311.  Perez-Piskunow PM, Usaj G, Balseiro CA, Fo`a Torres LEF. Floquet chiral edge states in graphene. Physical Review B 2014;89(12):121401. doi:10.1103/PhysRevB.89.121401.  Usaj G, Perez-Piskunow PM, Fo`a Torres LEF, Balseiro CA. Irradiated graphene as a tunable floquet topological insulator. Physical Review B 2014;90(11):115423.
doi:10.1103/PhysRevB.90.115423.  Huang YC, Lin MF, Chang CP.
Landau levels and magneto-
optical properties of graphene ribbons. 2008;103(7):073709.
Journal of Applied Physics
doi:10.1063/1.2902455.  Koshino M, Nakanishi T, Ando T. Interface landau levels in graphene monolayer-bilayer junctions. Physical Review B 2010;82(20):205436.
URL: ://WOS:000286736100005. doi:10.1103/PhysRevB. 82.205436.  Crommie MF, Lutz CP, Eigler DM.
Confinement of electrons to
quantum corrals on a metal-surface.
262.5131.218.  Ilani S, Martin J, Teitelbaum E, Smet JH, Mahalu D, Umansky V, et al. The microscopic nature of localization in the quantum hall effect. Nature 2004;427(6972):328. URL: ://WOS:000188266200034. doi:10.1038/nature02230.  Richardella A, Roushan P, Mack S, Zhou B, Huse DA, Awschalom DD, et al. Visualizing critical correlations near the metal-insulator transition in ga1-xmnxas. Science 2010;327(5966):665. URL: ://WOS: 000274251800031. doi:10.1126/science.1183640.  Crommie MF, Lutz CP, Eigler DM. a 2-dimensional electron-gas.
Imaging standing waves in
://WOS:A1993LF93900042. doi:10.1038/363524a0.  Rubio A, Sanchez-Portal D, Artacho E, Ordejon P, Soler JM. Electronic states in a finite carbon nanotube: A one-dimensional quantum box. Physical Review Letters 1999;82(17):3520. URL: ://WOS: 000079899900035. doi:10.1103/PhysRevLett.82.3520.  Jiang J, Dong JM, Xing DY. length metallic nanotubes.
Electronic properties in finite-
Physical Review B 2002;65(24):245418.
URL: ://WOS:000177043100104. doi:10.1103/PhysRevB. 65.245418. 44
 Lee J, Eggert S, Kim H, Kahng SJ, Shinohara H, Kuk Y.
space imaging of one-dimensional standing waves: Direct evidence for a luttinger liquid. Physical Review Letters 2004;93(16):166403. URL: ://WOS:000224533300060. doi:10.1103/PhysRevLett.93. 166403.  Hashimoto K, Sohrmann C, Wiebe J, Inaoka T, Meier F, Hirayama Y, et al. Quantum hall transition in real space: From localized to extended states. Physical Review Letters 2008;101(25):256802. URL: : //WOS:000261891200057. doi:10.1103/PhysRevLett.101.256802.  Miller DL, Kubista KD, Rutter GM, Ruan M, de Heer WA, Kindermann M, et al.
Real-space mapping of magnetically quantized
graphene states. Nature Physics 2010;6(10):811. URL: : //WOS:000283570000026. doi:10.1038/nphys1736.  Hashimoto K, Champel T, Florens S, Sohrmann C, Wiebe J, Hirayama Y, et al. Robust nodal structure of landau level wave functions revealed by fourier transform scanning tunneling spectroscopy. Physical Review Letters 2012;109(11):116805.
000308646600010. doi:10.1103/PhysRevLett.109.116805.  Fu YS, Kawamura M, Igarashi K, Takagi H, Hanaguri T, Sasagawa T. Imaging the two-component nature of dirac-landau levels in the topological surface state of bi2se3. Nature Physics 2014;10(11):815. URL: ://WOS:000344846700012. doi:10.1038/nphys3084.  Dresselhaus G, Dresselhaus MS. Fourier expansion for electronic energy bands in silicon and germanium. Physical Review 1967;160(3):649. URL: ://WOS:A19679823500027. doi:10.1103/PhysRev.160.649. 45
 Johnson LG, Dresselhaus G. Optical properies of graphite. Physical Review B 1973;7(6):2275. URL: http://link.aps.org/doi/10.1103/ PhysRevB.7.2275. doi:10.1103/PhysRevB.7.2275.  Lew Yan Voon LC, Ram-Mohan LR. Tight-binding representation of the optical matrix-elements - theory and applications. Physical Review B 1993;47(23):15500. URL: ://WOS:A1993LJ15400013. doi:10. 1103/PhysRevB.47.15500.  Gruneis A, Saito R, Samsonidze GG, Kimura T, Pimenta MA, Jorio A, et al. Inhomogeneous optical absorption around the k point in graphite and carbon nanotubes. Physical Review B 2003;67(16):165402. doi:10. 1103/PhysRevB.67.165402.  Jiang J, Saito R, Gruneis A, Dresselhaus G, Dresselhaus MS. Optical absorption matrix elements in single-wall carbon nanotubes. Carbon 2004;42(15):3169. doi:10.1016/j.carbon.2004.07.028.  Chiu CW, Lee SH, Chen SC, Shyu FL, Lin MF. Absorption spectra of aa-stacked graphite. New Journal of Physics 2010;12:083060. URL: ://WOS:000281489700004. doi:10.1088/1367-2630/ 12/8/083060.  Ho YH, Chiu YH, Lin DH, Chang CP, Lin MF. Magneto-optical selection rules in bilayer bernal graphene. ACS Nano 2010;4(3):1465. doi:10.1021/nn9015339.  Huang YC, Chang CP, Lin MF.
Magnetoabsorption spectra of
bilayer graphene ribbons with bernal stacking. B 2008;78(11):115422.
 Sadowski ML, Martinez G, Potemski M, Berger C, de Heer WA. Landau level spectroscopy of ultrathin graphite layers. Physical Review Letters 2006;97(26):266405. URL: ://WOS:000243167300034. doi:10.1103/PhysRevLett.97.266405.  Poumirol JM, Yu W, Chen X, Berger C, de Heer WA, Smith ML, et al. Magnetoplasmons in quasineutral epitaxial graphene nanoribbons. Physical Review Letters 2013;110(24):246803. URL: : //WOS:000320307500013. doi:10.1103/PhysRevLett.110.246803.  Berciaud S, Potemski M, Faugeras C. Probing electronic excitations in mono- to pentalayer graphene by micro magneto-raman spectroscopy. Nano Letters 2014;14(8):4548. doi:10.1021/nl501578m.  Robertson AW, Bachmatiuk A, Wu YA, Schaeffel F, Rellinghaus B, Buechner B, et al. Atomic structure of interconnected few-layer graphene domains. ACS Nano 2011;5(8):6610. doi:10.1021/nn202051g.